#------------------------------------------------------------------------------
#$Date: 2024-04-25 17:59:02 +0300 (Thu, 25 Apr 2024) $
#$Revision: 291351 $
#$URL: file:///home/coder/svn-repositories/cod/cif/9/00/28/9002830.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the American Mineralogist Crystal Structure Database,
# http://rruff.geo.arizona.edu/AMS/amcsd.php
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_9002830
loop_
_publ_author_name
'Redhammer, G. J.'
'Roth, G.'
_publ_section_title
;
 Single-crystal structure refinements and crystal chemistry of
 synthetic trioctahedral micas KM3(Al,Si)4O10(OH)2, where
 M = Ni, Mg, Co, Fe, Al
 Sample: Coni1.8#2 - Co
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1464
_journal_page_last               1476
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Al1.08 Co1.68 H2 K Ni1.32 O12 Si2.92'
_chemical_name_mineral           Phlogopite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 99.949
_cell_angle_gamma                90
_cell_length_a                   5.3225
_cell_length_b                   9.2195
_cell_length_c                   10.3125
_cell_formula_units_Z            2
_cell_volume                     498.433
_database_code_amcsd             0002919
_exptl_crystal_density_diffrn    3.470
_cod_original_formula_sum        '(Al1.08 Si2.92) (Co1.68 Ni1.32) K O12 H2'
_cod_database_code               9002830
loop_
_space_group_symop_operation_xyz
x,y,z
1/2+x,1/2+y,z
x,-y,z
1/2+x,1/2-y,z
-x,y,-z
1/2-x,1/2+y,-z
-x,-y,-z
1/2-x,1/2-y,-z
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_U_iso_or_equiv
AlT 0.57637 0.16674 0.22848 0.27000 0.00811
SiT 0.57637 0.16674 0.22848 0.73000 0.00811
CoM1 0.00000 0.50000 0.50000 0.56000 0.00874
NiM1 0.00000 0.50000 0.50000 0.44000 0.00874
CoM2 0.00000 0.83190 0.50000 0.56000 0.00887
NiM2 0.00000 0.83190 0.50000 0.44000 0.00887
K 0.00000 0.00000 0.00000 1.00000 0.03318
O1 0.82794 0.22891 0.17079 1.00000 0.02128
O2 0.51410 0.00000 0.17080 1.00000 0.02140
O3 0.63136 0.16663 0.39129 1.00000 0.01039
O4 0.13362 0.00000 0.39809 1.00000 0.01102
H 0.11100 0.00000 0.28800 1.00000 0.02976
loop_
_cod_related_entry_id
_cod_related_entry_database
_cod_related_entry_code
1 AMCSD 0002919
